Segregation of Sublattice Domains in Nitrogen-Doped Graphene Amir Zabet-Khosousi,† Liuyan Zhao,‡ Lucia Pálová,† Mark S. Hybertsen,§ David R. Reichman,† Abhay N. Pasupathy,‡ and George W. Flynn*,† †
Department of Chemistry, Columbia University, New York, New York 10027, United States Department of Physics, Columbia University, New York, New York 10027, United States § Center for Functional Nanomaterials, Brookhaven National Laboratory, Upton, New York 11973, United States ‡
S Supporting Information *
ABSTRACT: Atomic-level details of dopant distributions can signiﬁcantly inﬂuence the material properties. Using scanning tunneling microscopy, we investigate the distribution of substitutional dopants in nitrogen-doped graphene with regard to sublattice occupancy within the honeycomb structure. Samples prepared by chemical vapor deposition (CVD) using pyridine on copper exhibit well-segregated domains of nitrogen dopants in the same sublattice, extending beyond 100 nm. On the other hand, samples prepared by postsynthesis doping of pristine graphene exhibit a random distribution between sublattices. On the basis of theoretical calculations, we attribute the formation of sublattice domains to the preferential attachment of nitrogen to the edge sites of graphene during the CVD growth process. The breaking of sublattice symmetry in doped graphene can have important implications in its electronic applications, such as the opening of a tunable band gap in the material.
INTRODUCTION Substitutional doping of a crystal oﬀers a robust approach for modifying the crystal’s properties, through the introduction of foreign atoms into the host lattice structure.1,2 However, in addition to the structure and composition of individual dopants, the spatial distribution of the dopants also constitutes an important factor that can be used to control material properties.3 For example, in nanoscale semiconductor devices, ordered versus randomly distributed dopants have been shown to signiﬁcantly enhance device performance.4 Therefore, atomic-level control over dopant distributions provides an important characteristic to be considered in the development of functional nanomaterials. With recent advances in the formation of two-dimensional materials such as graphene, and its chemical doping with foreign atoms (e.g., nitrogen),5−10 there now exists an unprecedented opportunity to investigate the distribution of dopants in two dimensions with atomic-scale spatial precision. Recently, we showed that individual dopants in graphene can be visualized using scanning tunneling microscopy/spectroscopy (STM/STS),11,12 which provides both subatomic spatial resolution and compositional sensitivity through the measurement of electron tunneling characteristics at the surface.13 In our previous studies, nitrogen-doped graphene was prepared on polycrystalline copper foil by chemical vapor deposition (CVD) from mixtures of methane and ammonia,11 and because of the roughness of the copper-foil substrate, our initial attempts to study the distribution of dopants in these samples were limited to small scan areas, typically 30 nm × 30 nm. Nevertheless, our previous STM measurements revealed an unusual sublattice segregation of nitrogen dopants; of the two graphene © XXXX American Chemical Society
sublattices, nitrogen dopants were found to predominantly occupy only one sublattice.11,12 However, in certain other studies of nitrogen-doped graphene, 14,15 the sublattice segregation is not clearly observed. There are thus several open questions about dopant sublattice segregation, including the conditions under which it can be observed, the length scale of the segregated domains, and a microscopic understanding of the mechanism that drives the observed eﬀect. Here, in order to answer these questions, we have modiﬁed the graphene growth method by using single-crystal Cu(111) substrates, which allowed us to achieve large, atomically ﬂat terraces of as-grown graphene, thus enabling investigations of dopant distributions on a large scale while maintaining atomic spatial resolution. Using these substrates, we have performed a systematic set of measurements to probe the inﬂuence of various sample-preparation conditions on the dopant sublattice distribution, and used density functional theory (DFT) to gain insight into the segregation process. Our present STM measurements reveal large (up to 100 nm in size) well-separated domains where nitrogen dopants are located on the same sublattice. These sublattice domains are only present in samples grown by CVD, whereas other methods of nitrogen dopingsuch as reaction with ammonia or nitrogen ion bombardmentyield random distributions of sublattices. On the basis of DFT calculations, we attribute the observed segregation of sublattice domains in the CVD samples to the way in which the nitrogen atoms are incorporated into the graphene lattice during the growth process. Our ﬁndings, Received: August 27, 2013
dx.doi.org/10.1021/ja408463g | J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
Journal of the American Chemical Society
thus, provide new insights into the mechanism of graphene growth. Furthermore, the presence of doped sublattice domains could have important implications for extending the electronic applications of graphene through, for instance, band gap engineering.
RESULTS AND DISCUSSION
Preparation of Cu(111) with large atomic terraces was performed in an ultrahigh vacuum (UHV). The conventional CVD scheme for growing graphene was modiﬁed to take into account the UHV conditions,16 in particular by replacing the precursor mixture of methane and ammonia with pyridine (C5H5N) as a single source of carbon and nitrogen.17,18 The use of a large precursor molecule also allowed us to lower the precursor pressure to ∼1 mTorr (compared to ∼1 Torr for the conventional CVD growth), which is more compatible with the UHV environment. Figure 1a shows an atomically resolved STM image of a CVD-grown nitrogen-doped sample. As reported previously,11,14,15,19 the graphitic nitrogen dopants appear dark in STM images, whereas the carbon atoms adjacent to nitrogen appear bright due to an increase in the local density of states (DOS). The unit cell of graphene consists of two carbon atoms, each occupying one of the two sublattices (A or B) that together constitute the honeycomb lattice of graphene. These sites are equivalent by symmetry in pristine graphene.20 However, when carbon atoms are substituted by dopants, these two sublattices can behave diﬀerently. Simulated STM images, Figure 1b, show that charge transfer from nitrogen to graphene is maximized for carbon atoms that are located on the sublattice opposite to that containing nitrogen. These carbon atoms together form a triangle encompassing the bright region surrounding the nitrogen. Depending on the original sublattice position of the dopant, these triangular features appear as mirror images of each other, as illustrated by red and blue triangles in Figure 1b. This behavior thus allows us to resolve the sublattice position of each dopant in STM images; examples are highlighted in Figure 1a. Figure 1c shows the STM topography of a larger area (20 nm × 20 nm) on a CVD-grown sample. Two important observations are noteworthy: First, the concentration of nitrogen dopants in the sample is 0.18%, which is much smaller than the original content of nitrogen in the precursor pyridine, 17%, indicating that the growth does not occur molecule by molecule; rather, the precursor breaks down into small fragments containing C or N. The growth of graphene then involves diﬀusion of these fragments on the surface until they reach a growing seed. The smaller content of nitrogen in graphene than in the precursor suggests that nitrogen, compared to carbon, either diﬀuses more slowly on the Cu(111) surface or reacts at a lower rate with graphene (the diﬀerence is ∼100-fold in this case), or nitrogen has a shorter lifetime at the surface due to competing pathways such as migration into the copper substrate or desorption via formation of N2. We note that the dopant concentration in the pyridinegrown samples is comparable to that in ammonia/methane grown samples,11 indicating that similar growth mechanisms are operating in both cases. The second striking observation is that all nitrogen dopants in Figure 1c are located on the same sublattice. This behavior clearly contradicts the natural expectation of random dopant
Figure 1. STM images of nitrogen-doped graphene. (a) STM image (7 × 7 nm2, 1 V, 1 nA) of nitrogen-doped graphene on Cu(111) showing three dopants on two diﬀerent sublattices. Bright colors in the STM image (red and yellow) correspond to carbon atoms surrounding nitrogen dopants, and red and blue triangles indicate dopants on diﬀerent sublattices. (b) Simulated STM images of graphitic nitrogen dopants located on two diﬀerent sublattices. Green diamonds indicate the unit cell of graphene, and black and white circles indicate the sublattices. Carbon atoms in the vicinity of the nitrogen dopants appear bright (red and yellow), forming triangles that appear as mirror images for the two sublattices (highlighted by red and blue triangles). (c) STM image (20 × 20 nm2, 1 V, 1 nA) of CVD(pyridine)-grown nitrogen-doped graphene, showing all dopants located on the same sublattice. B
dx.doi.org/10.1021/ja408463g | J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
Journal of the American Chemical Society
Figure 2. Distribution of nitrogen dopants in CVD(pyridine)-grown doped graphene. (a) STM image (100 × 100 nm2, 1 V, 1 nA) of CVD-grown doped graphene on Cu(111). Dopant sublattices are highlighted by red (A) and blue (B) triangles. Scale bar = 10 nm. (b) Spatial analysis of sublattice distribution. ▼ = sublattice A. △ = sublattice B. fA (or f B) represents the fraction of dopants in sublattice A (or B) within a local radius. The color scale represents fA and f B and ranges from 0.5 (white) to 1 (red and blue for A and B, respectively). ⟨dN−N⟩ = average interdopant separation. ⟨f⟩ = average degree of sublattice segregation. (c) Map of p-values corresponding to the ratios shown in map b, obtained under a null hypothesis.
rejected with a conﬁdence level greater than 99%. These green domains clearly constitute the dominant portions of the map. Interestingly, the size of the domains extends over 100 nm, and also there is a sharp boundary between the domains with a width of ∼1 nm, smaller than the average interdopant separation, ⟨dN−N⟩ = 2 nm. Note that the boundary between the sublattice domains is independent of the structural grain boundaries in graphene. The image in Figure 2a involves a single lattice orientation of graphene, as evidenced by the observation of a uniform Moiré pattern21 in the background. Further examples of sublattice domains in the CVD samples are shown in the Supporting Information, Figure S1, demonstrating the generality of this observation. To investigate the cause of sublattice segregation, we examined a number of diﬀerent methods for producing nitrogen-doped graphene. These included postsynthesis treatment of pristine graphene, by (a) reaction with ammonia or (b) nitrogen ion bombardment.22,23 Figure 3 shows maps of dopant distributions resulting from these two methods, and they exhibit essentially a random distribution of sublattices, as evidenced by small degrees of segregation, ⟨f⟩ < 60%, and absence of continuous domains of p-values